Presentation on theme: "Systematic Errors and Sample Preparation for X-Ray Powder Diffraction"— Presentation transcript:
1 Systematic Errors and Sample Preparation for X-Ray Powder Diffraction Jim ConnollyEPS , Spring 2010
2 IntroductionMost systematic errors in diffraction experiments are related to the characteristics, preparation and placement of the specimen. Today we will:Differentiate and define those errorsPresent preparation techniques to minimize those errorsDiscuss different types of sample mounting strategies and trade-offs of various methodsAlways remember the distinction between sample and specimenFootnote question: What is the difference between a random and systematic error?
3 Goals of Specimen Preparation Overall Rule: The time and effort put into specimen preparation should not be more than is required by the experiment objectiveBasic information in the diffraction pattern:The position of the diffraction peaksThe peak intensities, and shape of peaksThe intensity distribution as a function of diffraction angleThe utility of this information depends on both the experiment parameters and the sample preparationCommunicate with your “client” about the objectives of your experimentDesign your experiment to achieve those objectives
4 Specimens and Experimental Errors Axial Divergence: The X-ray beam diverges out of the plane of the focusing circleFlat Specimen Error: The specimen is flat, and does not follow the curvature of the focusing circle.Compositional Variations between Sample and SpecimenSpecimen Displacement: Position of the sample mount causes deviation of the focusing circleSpecimen Transparency: Beam penetration into a “thick” specimen changes diffraction geometrySpecimen Thickness: Trade-offs between accuracy of peak positions and intensitiesParticle Inhomogeneity: Can significantly alter diffraction intensitiesPreferred Orientation: Can produce large variations in intensity and limit the peaks seen.
5 Beam Path from Source to Detector Path from X-ray source to detector is shown at rightBeam path:From horizontal source F tovertical soller slits SS1 toDivergence slit D5Specimen S (A=center of diffractometer circle) toReceiving Scatter slit RS toReceiving soller slits SS2 toscatter slit SS toMonochromator and Detector (not in picture)
6 Axial DivergenceDetector sees the arc of the Debye ring not just the diffractions along the 2D diffractometer circleLeads to a notable peak asymmetry, particularly pronounced at low 2θAxial Divergence error for Silver Behenate is shown at rightCan be minimized by closely spaced soller slits (at the cost of reduced intensity)
7 Flat Specimen ErrorThe extreme edges of the specimen lie on another focusing circle (rf’) which results in the overall diffracted intensity being skewed to a lower value of 2.This is related to the divergence of the incident beam by the equation below where is the angular aperture of divergence slit in degreesDiv Slit2minMoKCuKCrK0.254.68.8619.2428.580.509.24.455.6114.351.0018.42.224.837.182.0037.21.112.423.594.0078.00.561.221.81The table at right shows specimen irradiation lengths (in mm) for a diffractometer of a particular radius (not ours)
8 Differences between Sample and Specimen Grinding EffectsProblem: Excessive percussive grinding produces extremely small particle size peak broadeningRemedy: Be careful (or use non-percussive grinding techniques)Irradiation EffectsInteraction with beam changes specimenRare in inorganics; significant issue in organics and phases with poorly-bound H2OEnvironmental EffectsStrain effects in materials at elevated temperatureChemical reactivity of specimenSensitivity to water, air or other solventsUsually reversible, sometimes notSystematically used as a tool in clay analysis
9 Specimen Displacement Cause: Specimen is higher or lower than it should be (i.e., not at center of diffractometer circle or tangent to focusing circle)Effect: 2θ error defined by the following equation:(R is the radius of the diffractometer circle; s is the deviation from the correct position on the focusing circle measured as the difference between r and r’)Can be a significant cause of errors in 2θMore pronounced at low θ values (cosine function)Can produce asymmetric peak broadening at low angles (resembling axial divergence)2θ can be as much as 0.01º for each 15m of displacement at low anglesCan be caused by poor diffractometer alignment
10 Specimen Transparency Caused by diffraction occurring at depth within a thick specimenResults in 2θ related to effective penetration depth of the specimenThe error is defined: is dependent on mass and the x-ray wavelengthFor SiO2 and CuK, = 97.6/cm, or approx. 100/cm. Thus t0.5 thus is about 0.01 cm or 100 m.For high-density, high / materials (metals, alloys), t0.5 will be on the order of 10 mFor low-density organics, t0.5 will be on the order of 1,000 m, and a thick sample will induce very significant displacement errorsLoose packing of powders can add reduce density and thus increase t0.5where is the linear attenuation (a.k.a. linear absorption) coefficient for the x-ray wavelength, R is the radius of the diffractometer circle and 2 is in radiansDefines the working depth
11 Specimen Thickness Bottom line for specimens is: Thin specimens Yield the best angular measurements (i.e. most accurate peak positions)Do not yield accurate intensity measurements (because of bad particle statistics)Tend to be more susceptible to preferred orientation effectsThick specimensCan yield good intensity measurements (better particle statistics, less susceptible to preferred orientation)Susceptible to angular measurement errors
12 Sample Inhomogeneity Multi-phase samples may be inhomogeneous In example at right chalcopyrite CuFeS2 (A) partially oxidized to cuprospinel CuFe2O4 (C)A and C have different mass attenuation coefficients ( and116.1, respectively)The result will be diffraction intensities from the two phases that are not directly proportional to the amounts of the phases presentThis effect is called the absorption effect or the particle inhomogeneity effect.
13 Preferred Orientation Preferred Orientation (lack of random orientation in the powder) is usually the dominant cause of intensity variations in a diffraction pattern.Effect is most pronounced for crystals with anisotropic shapes (or habits)This significantly affects the diffracted intensities from the specimen.
14 Preferred Orientation Occurs as a consequence of the “spotty” nature of diffraction in a non-random specimenThe effect is that the Debye ring is uneven in intensity
15 Preferred Orientation How the preferred orientation is manifest in the diffraction pattern varies with the materialClay minerals have a platy habit and will orient perpendicular to (00l).Equant cubes (NaCl) orient parallel to their cubic crystal facesBladed (most pyroxenes and amphiboles) or fibrous (most asbestos minerals and some zeolites) materials orient parallel to their elongation directionSome engineered polymers use preferred orientation for specialized qualitiesSevere preferred orientation in a specimen will result in “invisible” diffraction peaksIn most specimens, all of the diffraction peaks will be seen but their relative intensities will differ from the “ideal” pattern.Careful specimen preparation can minimize the effectWhole-pattern refinements can use preferred orientation as another parameter to be fit to the data
16 Particle StatisticsQuantitative (and semi-quantitative) X-ray powder diffraction is based on the principle that quantities are proportional to intensity.Accurate intensities require:Random orientation of crystallites in the specimenSufficient number of particles for good crystallite statisticsNote: Particle size is frequently (erroneously) equated with crystallite sizeAt right is a schematic pole plot of diffractions from two powder specimens on a sphereA random pattern indicates a random orientation
17 A particle statistics exercise It is instructive to understand how crystallite statistics will quantitatively affect intensity, i.e., what size particles are required to achieve a repeatability in intensity measurements?Assume a powdered quartz (SiO2) specimen:Volume = (area of beam) x (2x half-depth of penetration)Assume area = 1cm x 1cm = 100mm2t½ = 1/, where = linear absorption coefficientSiO2 = 97.6 /cm or ~100 /cm = 10 /mmV = (100) (2) / 10 mm3Thus Volume = 20 mm3Estimate number of particles at different particle sizes:Particle Diameter 40 m10 m1 mV/particle3.35 x 10-5 mm35.24 x 10-75.24 x 10-10Particles/mm32.98 x 1041.91 x 1061.91 x 109Particles in 20 mm35.97 x 1053.82 x 1073.82 x 1010
18 Particle Statistics Exercise (cont.) Equal distribution on a unit sphere (area = 4 steradians) yields a radiating sheaf of pole vectorsCalculating angular distribution on the sphere:Particle Diameter 40 m10 m1 mArea/pole, AP = 4/ # particles2.11 x 10-53.27 x 10-76.58 x 10-10Angle between poles, =0.2970.0370.005
19 Particle Statistics Exercise (cont.) Geometry of diffraction of a single particle:R is the diffractometer radius (a range is shown), F the focal length of the anode (a characteristic of the x-ray tube), and the angular divergence as shown. In the above example, L (= 0.5 mm) is the length of source visible to the target.NP (number of diffracting particles) = (area on unit sphere corresponding to divergence) / (area on unit sphere per particle) = AD/AP
20 Particle Statistics Exercise (cont.) To determine AD requires relating effective source area, FxL, to area on a unit sphere:= 2.5 x 10-4Calculating AD/AP yields the number of particles diffracting in any given unit area for our three particle sizes:Particle Diameter 40 m10 m1 mNP1276038,000Conclusion: The standard uncertainty in Poisson statistics is proportional to n½, where n is the number of particles. To achieve a relative error of < 1%, we need 2.3 = 2.3 n½ / n < 1%. This requires n > 52, 900 particles! Thus not even 1 m particles will succeed in achieving ±1% accuracy in intensity.The Bottom Line: Easily achievable particle sizes will not routinely yield high-precision, repeatable intensity measurements.
21 Enough of this Particle Statistics Stuff Other Factors can degrade or improve intensity accuracy:Concentration: mixed phase specimens reduce particles of a given phase in a unit area, increasing errorReflection multiplicity: Multiplicity in higher symmetry crystal structures give more diffraction per unit cell, improving statisticsSpecimen thickness: may improve diffraction volume, limited by maximum penetration depthPeak width (crystallite size): polycrystalline particles with random orientation can greatly improve statistics, but extremely small size will result in peak broadening.Specimen rotation/rocking: helps to get more particles in the beam. Rocking combined with rotation is best.Ultimately, quantitative analysis based on peak intensities cannot reliably achieve ±1% accuracy even under the most favorable specimen conditions of randomly oriented 1m particles
22 From Sample to Specimen From rock to powderBico Jaw Crusher * (Loc. 1)Plattner Steel Mortar & Pestle (Loc. 2)Spex Shatterbox * (Loc. 2)Mortar & Pestle (Loc. 2 & 3)Retch-Brinkman Grinder * (Loc. 3)Sieves for sizing (Loc. 2)* Manual for use available on class web pageEquipment Locations:1 – Northrop Hall Rm 1102 – Geochem Lab, Northrop Hall Rm 213 (see Dr. Mehdi-Ali)3 – XRD Lab, Northrop Hall Rm B-25
30 “Mesh” size of sieve screen Maximum diameter of particle passed To sieve or not to sieve . . .“Mesh” size of sieve screenMaximum diameter of particle passed20074 m32545 m40038 m60025 m100010 mSieves can be metal, teflon or other syntheticTheoretically 10 m particles may be passed (practically, it doesn’t work)Because of static forces, 325 mesh is smallest for routine use though 400 and 600 may be used with a lot of effort
31 Specimen MountsHow your specimen is mounted should be determined by the requirements of your experiment – i.e., don’t do more or less than is necessaryKnow the characteristics of your holder – always run your mount without any specimen to know your baseline “background” conditionsMount Types:Thin Mounts (best for accurate angular measurements)Slurry mounts (on any flat substrate)Double-stick tapePetroleum jelly “emulsion”Volume or “Bulk” Mounts (best for accurate intensity measurements)Side-drift mountsTop-load mountsThin-film mountsBack-pack mountsZero-background (off-axis quartz plate) mounts
32 Special techniques to reduce preferred orientation Aerosol Spray Drying using Clear Acrylic Lacquer (procedure outlined in class notes)Aqueous Spray Drying in a Heated Chamber (details at
33 After Spring Break on Mar 24: In-Class Exam: Coming Attractions:After Spring Break on Mar 24: In-Class Exam:Open-bookStart Promptly at 3:00 PM; do not be lateMust complete exam in 1 hourWritten short-answer formatAll reference materials okayTexts will be available for referenceIncludes everything through last week (Weeks 1 thru 6)Emphasis on demonstrating your understanding of materialFollowed by: Tour of the XRD LabLayout, location of all equipment and computersIntroduction to MDI DataScan program and scheduling of hands-on lab trainingRadiation safety exam should be completed before class